Md. Hasanuzzaman ID:2011000400007 1 | P a g e
Comparison of Tensile properties of Textile fibre
What is Tensile Properties:
A tensile property indicates how a material will react to the forces being applied in Tension.
Fibers usually experience tensile loads whether they are used for apparel or technical structures.
Their form, which is long and fine, makes them some of the strongest materials available as well
as very flexible. This book provides a concise and authoritative overview of tensile behavior of a
wide range of both natural and synthetic fibres used both in textiles and high performance
Tensile properties included
2) Elastic limit
4) Yield point
5) Breaking Extension
6) Elastic recovery. etc
Tensile properties are used to determine these properties.
The property of material of returning back to its original position after removing the external
force is known as elasticity. A body is known as elastic if its return back to its original shape and
size after removal the external force.
After deformation if the external force removed, the body springs back to its original position.
There is a limiting value of force, up to and within which the deformation entirely disappears on
removal of the force. The value of intensity of stress corresponding to this limiting force is called
elastic limit of the material.
After Elastic limit, when force increased the material loses to some extent of its property of
elasticity and cannot return to its original shape and size if the external force is completely
removed. In this condition the material gets into plastic stage and the property of the material is
known as plasticity
Fig: microscopic view of Textile fibres.
Md. Hasanuzzaman ID:2011000400007 2 | P a g e
When some external force acts on a body, It undergoes some deformation. As the body
undergoes deformation, it sets up some resistance to deformation. This resistance per unit area to
deformation is known as stress.
Mathematically stress may be defined as the force per unit area.
That is, S= F
S = Intensity of stress.
F = Load of force acting on the body.
A = cross sectional area.
Strain is the term used to relate the stretched or elongation with the initial length. The
deformation per unit length is known as strain.
Mathematically strain may be defined: E = I
E = strain.
I = change of length.
L = original length.
When a material is loaded, within the elastic limit, the stress is proportional to the strain.
Mathematically stress α strain
/ strain = K
When external force is applied to a material, it is balanced by internal forces developed in the
molecular structure of the material. By increasing the stresses, material will be deformed and
obey the stress-strain curve by the following way
Md. Hasanuzzaman ID:2011000400007 3 | P a g e
Region O to A:
Linear region, in this stage, the stress and strain initially increases with linear relations. This is
the linear-elastic portion of the curve and it indicates that no plastic deformation has occurred. In
this region of the curve, when stress is reduced, the material will return to its original shape, and
the line obeys the relationship defined as Hook’s law where the ratio of stress to strain is a
In this linear region (O to A) of the curve, the material behaves as perfectly elastic body and the
point ‘’A’’ indicates the ‘’Elastic Limit’’ of the material.
Region A to B:
After elastic limit, when stress is increased the material will notfollo9w the Hooks law. In this
region, strain is increased more with the increasing of stress and the material losses to some
extent of elasticity. If the external force, after causing deformation beyond the elastic limit, is
completely removed, the material will no return to its original shape and size and gets into plastic
The region (A to B) is called plastic region and the deformation is called plastic-deformation.
Region B to C:
In this region (B to C) for further increasing the stresses, the molecular chain of the material will
break down at the point.
The extension to break of a material to the initial length of that material is known as breaking
extension. It is expressed in percentage.
Breaking extension = X 100%
Md. Hasanuzzaman ID:2011000400007 4 | P a g e
Tensile Properties of different fibers is given below:
Table (Data) 1: Tensile properties of fibres at 65% r.h., 20 °C, 1 cm test length, 0.15mNtex–1
Fig 1: Stress–strain curves of various fibres tested at 65% r.h., 20 °C, 0.15mN tex–1
here Durafil is Lilienfeld rayon; Fibro is staple viscose rayon; Lanital is a casein fibre; acetate
rayon is secondary acetate.
Md. Hasanuzzaman ID:2011000400007 5 | P a g e
For the second generation of synthetic fibres, the high-modulus, high-tenacity fibres (HM–HT),
there is no comparative data for fibres tested in a single investigation. It is necessary to take data
from a variety of sources, for which test conditions may not be the same. A set of stress–strain
curves is shown in bellows chart. The complete collection of fibres can be roughly divided
mechanically into five groups. The weak inextensible fibres such as rock wool are of little
interest. The natural and regenerated fibres and some synthetics have moderate strength and
extensibility. The tough synthetic fibres have higher strength combined with extensibility. The
HM–HT fibres have high strength and low extensibility. The elastomeric fibres have low
tenacity, when related to their unstrained dimensions, and high extensibility.
Table (Data) 2: Tensile properties of some textile fibres at 65% r.h., 20 °C .
Md. Hasanuzzaman ID:2011000400007 6 | P a g e
Fig 2: Stress–strain curves of various fibres. Here viscose rayon variants are Fibro (regular
staple), Vincel (high-wet modulus) and Tenasco (high-tenacity, industrial); Terylene is polyester
fibre; Orlon is acrylic fibre.
Cotton and the other natural cellulose fibres:
The stress–strain curve for cotton is slightly concave to the extension axis, and there is no
obvious yield point. Meredith found considerable variation between different varieties of cotton.
In general, the finer cottons showed a higher tenacity and a higher initial modulus than the
coarser cottons. The breaking extension ranged from 5 to 10% but was not related to fineness.
Figure 5 shows stress–strain curves of five cottons from the 1970s. The Punjab–American cotton
is much stronger than the 1940s Bengals cotton in Table 1.
Meredith later showed that there was a better correlation between tenacity and molecular
orientation than there was between tenacity and fineness. The orientation may be measured by
the birefringence of the fibre, that is, the difference between the refractive indices for light
polarized parallel and perpendicular to the fibre axis. The orientation value decreases as the
spiral angle in the cotton fibre increases. Figure 6shows the correlation between tenacity and the
difference in the refractive indices for 36 different samples of cotton of 26 different varieties.
Md. Hasanuzzaman ID:2011000400007 7 | P a g e
Table (Data) 3: Tensile properties of HM–HT fibres from manufacturers’ literature.
Fig 3: Typical stress–strain curves of HM–HT fibres.
Md. Hasanuzzaman ID:2011000400007 8 | P a g e
Table (data) 4: Tensile properties of chemically and thermally resistant fibres.
Fig 4: Mechanical classification of the fibre types: A, HM–HT fibre; B, weak inorganic fibre,
e.g. rock wool; C, tough synthetic fibre; D, weaker textile fibre; E, elastomeric fibre.
Similar results are obtained by using X-ray methods to measure molecular orientation, and a
correlation is also found between initial modulus and orientation. It must, however, be noted that
it has been reported that the spiral angle of cotton fibres is constant within the range 20–23° and
that the apparent differences are really due to the effect of convolutions. Hessler et al.
investigated the effect of the length of chain molecules in the cotton and found that this also gave
a good correlation with the tenacity of different types of cotton. Thus it is not clear which is the
effective factor in determining the tenacity of different varieties of cotton. Morlier et al.
investigated the difference between fibres within a given sample of cotton for six different
varieties of cotton. In most cases, they found that tenacity and breaking extension increased with
increasing length of fibre.
Md. Hasanuzzaman ID:2011000400007 9 | P a g e
Fig5: Stress–strain curves for various cottons.
Fig 6: Correlation between tenacity and birefringence of cotton at test lengths of 1 mm and 1
An example of their results is given in Fig7. Meredith found no correlation between strength and
fineness within a sample of cotton. Timpa and Ramey found an increase ofstrength, measured in
four laboratories according to HVI standards, from 0.2 to 0.3 N/tex with increasing length from
21.2 mm (staple length code: 26) to 32 mm (code: 40); they also found a significant increase of
strength with molecular weight, albeit with considerable scatter.
Fig 7: Correlation between tenacity and length for a Sea Island cotton.
Md. Hasanuzzaman ID:2011000400007 10 | P a g e
Table (Data) 5: USDA descriptive designations for HVI tenacity values of cotton.
Foulk and McAlister report an extensive study of the tensile properties of cottons with three
micronaire values, each subdivided into seven length groups. With the advent of HVI testing of
cotton, the US Department of Agriculture (USDA) has given the designations of tenacity values
in Table as an indication of cotton fibre quality. Hearle and Sparrow studied the effect of
convolutions on the behaviour of cotton fibres. If a fibre is stretched, the convolutions are pulled
out. If the fibre is extended in the wet state and dried while held under tension, the extended form
is temporarily set. Figure 8 shows the effect on the stress–strain curve at 65% r.h. The treated
fibre is stiffer, and shows a higher tenacity and lower break extension.
The bast fibres, in which the molecules are very nearly parallel to the fibre axis, show a greater
tenacity, a higher modulus, a lower breaking extension and a lower work of rupture. They
constitute the strongest but least extensible of natural fibres. The jute tested by Meredith gave
lower values of tenacity than the other bast fibres, but it has been shown by Mukherjee et al. that
better-quality jute has a tenacityof 0.56 N/tex under similar conditions.
Md. Hasanuzzaman ID:2011000400007 11 | P a g e
Fig 8: Load–extension curves of Acala cotton: A, normal fibre; B, after stretching wet and
This is as strong as flax or hemp. Franck includes a large collection of reported values of
mechanical properties of bast and other plant fibres. The values are generally similar to those for
flax, jute, hemp and ramie in Data 1(Table 1).
Regenerated cellulose and related fibres:
The stress–strain curves of rayon and acetate fibres show an initial rapid rise with a marked yield
point, followed by a nearly flat portion and a rise again as breakage approaches. The curves vary
widely for different types of rayon and different manufacturing methods. Differences are due to
the spinning method and the degree of stretch imposed. A highly stretched fibre, such as the
formerly produced Durafil, has high molecular orientation, which gives high strength and low
extensibility, similar to the bast fibres. Rayons used for apparel are weaker and more extensible.
Tyre-cord rayons, such as Tenasco, are intermediate in value. The effect of orientation is clearly
shown in the set of curves in Fig. 9, for acetate of varying degrees of orientation. If cellulose
yarns are regenerated from the acetate, as they were in Fortisan, the locus of strengths is
somewhat higher. Acetate fibres are, in general, weaker and more extensible than viscose rayon
fibres. The load–elongation curves of acetate fibres, measured at constant rate of elongation,
often show a drop after the yield point.
Md. Hasanuzzaman ID:2011000400007 12 | P a g e
Fig9: Stress–strain curves of filaments of varying degrees of orientation. The dotted curves are
secondary cellulose acetate and the full curves are cellulose fibers regenerated from acetate.
There are also important differences in the tensile properties of viscose rayon,depending on their
fine structure. An improvement in structure will cause the whole locus of breaking points to be
moved farther from the origin, so that strength is increased without the loss of extensibility that
occurs when orientation is increased. This is illustrated in Fig. 10, and the great advances that
were made in hightenacity rayon tyre yarns in the 1950s are shown in Table 6. More extensible
analogues of these fibres are used as high-strength staple fibres. Rayons made until the 1950s
had a micellar structure, which results in a low-wet-modulus and a low strength. The modal
rayons, which include polynosic fibres, are fibrillar in texture, and are stiffer, and closer to cotton
in properties, than earlier rayon fibres. They have a high-wet-modulus and better wet strength.
The reasons for this are discussed in Section 20.2.2. Lyocell fibres, such as Tencel, are similar in
tensile properties, but somewhat stronger and stiffer. White et al. give dry tenacities and break
extensions of 0.38–0.42 N/tex at 14–16% dry and 0.34–0.38 N/tex at 16–18%. Chamberlain and
Khera  investigated the variation in the properties as the outer layers of viscose and
cuprammonium rayon filaments are removed chemically. A typical result for viscose rayon is
shown in Fig. 12. 1t appears from these results that the outermost layers are less extensible than
the layers below the surface, but the variation in tenacity cannot be worked out.
Md. Hasanuzzaman ID:2011000400007 13 | P a g e
Fig10: Load–extension curves for viscose rayon, showing changes produced by increasing
orientation and improving structure.
Table (Data) 6: Properties of viscose rayon tire cords.
Since the stress would concentrate in the least extensible parts of the fibre. The results for
cuprammonium rayon were different for the two samples of fibre tested. From reports by
different workers, Muri and Brown include tenacities N/tex and break extensions of 0.154/14.5%
and 0.183/ 6% for calcium alginate fibres and 0.204/10% for zinc alginate.
Silk, like nylon, is characterised by fairly high strength and breaking extension, which combine
to give a work of rupture very much greater than that of the other fibres tested by Meredith. The
wide range of spider silks include fibres of very high strength combined with high extensibility,
which leads to very high work of rupture.
Md. Hasanuzzaman ID:2011000400007 14 | P a g e
Fig 11: Stress–strain curves of lyocell (Tencel), modal and regular viscose rayon compared with
Fig 12: Change of tenacity and braking extension of viscose rayon as outer layers are removed.
Wool and other hair fibres are characterised by low strength but great extensibility. Owing to the
high breaking extension, and to the shape of the curve, the work of rupture is not low despite the
low strength. Different types of wool give slightly different curves, but these are always
characterised by an initial linear Hookean region up to 2% extension, a yield region of very low
slope from 2 to 30% extension, and finally a post-yield region of greater slope, up to a breaking
extension around 45%. The very extensive experimental studies that have been carried out on
wool have been reviewed by Chapman and Feughelman .Much of the work has beendone on wet
fibres, and Collins and Chaikin have found that, if the effects of fibre irregularity are eliminated,
the separate regions become even more distinct, with sharp turning points between them, and the
yield slope becomes very small.
Regenerated protein fibres are weak and extensible and even weaker when wet. In addition to the
fibres manufactured in the 1950s, this also applies to the attempts to produce fibres from spider
silk proteins derived from genetically engineered sources.
It is important to known about textile fibres tensile properties for having a better idea about
textile fiber. By doing this assignment I got a brief idea about tensile properties of textile fibre.
Md. Hasanuzzaman ID:2011000400007 15 | P a g e
Class lecture, Delivered by Mr. Nazmul Ehsan
1) Physical properties of textile fibres (Fourth edition), By- W. E. Morton and J. W. S.